By Zachary Zguris, PhD
FORMLABS WHITE PAPER:
How Mechanical Properties of Stereolithography 3D Prints are Affected by UV Curing
FORMLABS WHITE PAPER: How Mechanical Properties of Stereolithography 3D Prints are Affected by UV Curing 2
The post-cure of parts printed with Formlabs resins on the Form 1+ and Form 2 printers was thoroughly
investigated. From the results, we are now able to recommend post-cure procedures for Castable, Standard,
and Tough Resins that provide the highest mechanical properties. In all cases, a 405 nm light source during
post-cure is superior to an equivalent level of lower wavelength light, such as 365 nm. Counter to the common
belief that more light results in better post-cured properties, the optimum flux on a printed part needed
to obtain maximum mechanical properties during post-cure has been determined to be 1.25 mW/cm2. It
was found that post-curing at higher temperatures results in a shorter time to full cure. Additionally, higher
temperatures lead to higher mechanical properties. A complete list of recommended post-cure times and
temperatures for all of Formlabs resins is provided.
Prior to this work, there had been little scientific study about post-curing prints made on Formlabs desktop
SLA 3D printers. The Formlabs line of SLA resins includes a series of Standard Resins: Clear, White, Grey,
and Black. In addition to the Standard Resin family, Formlabs offers Functional Resins: Tough, Castable, and
Flexible. Each resin is a finely-tuned proprietary formulation developed and engineered from the ground up
to work with the Form 1, Form 1+ and Form 2 SLA 3D printers. These machines all use a 405 nm laser. All of
the Formlabs resins are tailored to this wavelength.
Other manufacturers of SLA 3D printing resins design their products for use with differing wavelengths,
chemistries, and print processes. Recommended post-cure procedures for other brands of 3D printing resins
are not likely to work with Formlabs resins for best results. To date, Formlabs recommendation for print
post-curing is based on generally accepted post-cure practices in the industry.
After realizing that Formlabs resins are each a unique formulation engineered to work specifically with our
printers, we set out to study the post-cure process in detail with the singular goal of developing the best
possible post-cure procedures for our users. To this end, the effects of the post-cure process parameters of
temperature, wavelength, time, and radiant flux on the mechanical properties of prints made using Formlabs
printers and resins were studied.
Experiments were designed to determine the effect of the individual post-cure process parameters of
temperature, wavelength, time, and flux. The experimental setups were designed to eliminate all controllable
variables outside of the specific one being studied in each set of experiments.
All of the mechanical data was acquired with a Test Resources Universal Testing Machine (Model 500LB
Actuator, Model SM-500-294 Load Cell, Epsilon Technology Corp. Axial Extensometer Model 3542-0100-
050-ST). ASTM D638 type IV tensile bars were used as the standard printed part throughout this research.
In all plots, the error bars report standard deviation for the mean of four samples.
Both Form 1+ and Form 2 printed ASTM D638 type IV tensile bars were used for experimental samples. All
of the data presented, unless otherwise indicated, is for samples printed using Formlabs Clear V2 Resin at
a 100-m layer height. The samples were manually oriented at 45 degrees in the x direction and 0 degrees
in the y direction. Supports were carefully edited in PreForm software to eliminate any defects in the necked
region caused by support touch points. The orientation used to print tensile bars is illustrated in Figure 1.
FORMLABS WHITE PAPER: How Mechanical Properties of Stereolithography 3D Prints are Affected by UV Curing 3
Time, temperature, and wavelength experiments were all performed on the same experimental apparatus,
shown in Figure 2. This cure study apparatus (CSA) is composed of a heat sink with a mounted 10W LED
array supported a fixed distance over tensile bar samples located in a transparent acrylic holder over a
reflective aluminum surface. A fan blows continuously over the samples to maintain a constant uniform
sample temperature. The CSA frame is an open structure to facilitate air movement over samples. The CSA
frame locates the LED array in a central position a fixed distance of 90 mm over the samples. An acrylic
sample holder positions each of four tensile samples to eliminate positional variation. The uniformity of the
light over the sample holder was verified. No variations in mechanical properties due to sample location
were found. Additional equipment used consisted of a four-channel Type K thermocouple data logger
(Measurement Computing model USB-TC) and an Auber-WS PID temperature controlled CADCO XAF013 Oven.
Figure 1: PreForm Orientation of ASTM Type IV Tensile Bars
Figure 2: Cure Study Apparatus
FORMLABS WHITE PAPER: How Mechanical Properties of Stereolithography 3D Prints are Affected by UV Curing 4
Flux experiments at 405 nm were carried out in a separate test cure chamber (TCC) built specifically for
further post-cure research and study. The TCC was built to allow control of the amount of 405 nm light the
test samples were exposed to during post-cure. This second apparatus consists of an insulated chamber
with multiple light sources, a convection heater, temperature control, time control, and a locating sample
holder as shown in Figure 3. The TCC allowed for the control of one to four 10W LED arrays in addition to a
3.2W star puck LED. This apparatus was used to determine the effects that differing levels of radiant power
incident on a post-curing parts surface had on mechanical properties.
Light sources consisted of 10W LED arrays from Shenzhen Yonton Opto Company with the three different
output wavelengths of 365 nm, 385 nm, and 405 nm. Because it was not readily possible to control the luminous
power of each array, the input power into the LED array was fixed and held constant by a commercial LED
driver (Shenzhen Yonton Opto Co. model: 10W[3x3]). Each LED array was powered by the same 10W constant
current DC power source. All of these components were from a single source supplier. Each chip was identical
in form factor and input power. In addition to the three LED arrays, a 9W 365 nm UV Fluorescent bulb (UV-9W
365 nm) was also investigated. A Thorlabs UV-Vis spectrometer (model: CCS100) was used to quantify the
wavelength produced by each light source. A Thorlabs Digital Handheld Optical Power and Energy Meter
Console (model: PM100D) with 5 mm dia integrating sphere (model: S140C) was used to quantify the flux.
Figure 3: Post-Cure Chamber Used for Radiant Flux Experiments
TABLE 1: MEASURED OUTPUT OF LIGHT SOURCES
Array Wavelength (nm) Peak Wavelength (nm) Power (mW)
405 406.9 3.41
385 389.2 1.61
365 368.1 1.17
Fluorescent 365 366 0.923
FORMLABS WHITE PAPER: How Mechanical Properties of Stereolithography 3D Prints are Affected by UV Curing 5
The evaluation of the light sources is summarized in Table 1. Results verify that each light source produces
light near enough to the specified wavelength but to differing efficiencies for the same input power of 10W.
Figures 4 through Figure 7 show the spectra for each light source. The LED arrays produce similar peaks
around but slightly above the reported nominal value of the array. The 9W UV fluorescent bulb shows a
broader peak around 365 nm in addition to the expected Mercury spectrum overlay.
Figure 4: Spectrum of 365 nm 10W LED Array
Figure 6: Spectrum of 405 nm 10W LED Array
Figure 5: Spectrum of 385 nm 10W LED Array
Figure 7: Spectrum of 365 nm 9W Fluorescent Bulb
FORMLABS WHITE PAPER: How Mechanical Properties of Stereolithography 3D Prints are Affected by UV Curing 6
RESULTS AND DISCUSSION:
Our study of the effects of three wavelengths, 365 nm, 385 nm, and 405 nm, on the post-cured mechanical
properties of printed parts showed a distinct difference. The results of these experiments are shown in
Figures 8 and 9.
We find that the best modulus and tensile strength are developed by post-curing with a 405 nm light source.
With a post-cure of 120 minutes and 44 C, the modulus at 365 nm is only 67% that of the 405 nm samples.
There is a significant difference in the post-cured properties at each wavelength, especially so at shorter
post-cure times. This is not surprising given that Formlabs resins are designed to work with the Form 1,
Form 1+, and Form 2 printers, all of which use a 405 nm laser. While 365 nm and 385 nm light both produce
post-cured modulus and tensile strengths that are higher than uncured green state samples shown at t=0,
neither approach the properties obtained with a 405 nm source post-cure.
Figure 8: Effect of Clear V2 Post-Cure Wavelength on Ultimate Tensile Strength
Figure 9: Effect of Clear V2 Post-Cure Wavelength on Modulus
FORMLABS WHITE PAPER: How Mechanical Properties of Stereolithography 3D Prints are Affected by UV Curing 7
The effect of temperature on the post-cured modulus